# Piezo ceramics.pdf

Piezo ceramics.pdf

Piezo ceramics.pdf

### You also want an ePaper? Increase the reach of your titles

YUMPU automatically turns print PDFs into web optimized ePapers that Google loves.

<strong>Piezo</strong> <strong>ceramics</strong><br />

Noliac Group develops and<br />

manufactures piezoelectric<br />

<strong>ceramics</strong> based on modified lead<br />

zirconate titanate (PZT) of high<br />

quality and tailored for custom<br />

specifications.<br />

<strong>Piezo</strong>electric <strong>ceramics</strong> may be used to produce e.g.:<br />

• Actuators<br />

• Sensors<br />

• Generators<br />

• Transducers<br />

www.noliac.com <strong>Piezo</strong> <strong>ceramics</strong> Ver0901 1

<strong>Piezo</strong> <strong>ceramics</strong><br />

<strong>Piezo</strong> <strong>ceramics</strong> specifications<br />

Properties Symbol & unit NCE40 NCE41 NCE46<br />

*<br />

NCE51 NCE53 NCE55 NCE57<br />

*<br />

NCE59<br />

*<br />

NCE80<br />

DIELECTRIC PROPERTIES (tolerances +/- 10%)<br />

Relative Dielectric Constant<br />

ε T 33<br />

ε 0<br />

1250 1350 1300 1850 1600 5000 1800 2900 1050<br />

Dielectric Loss Factor tgδ [10 -4 ] 25 40 30 190 130 220 170 190 20<br />

Dielectric Loss Factor at 400V/mm tgδ [10 -4 ] 140 200 100<br />

ELECTROMECHANICAL PROPERTIES (tolerances +/- 5%)<br />

Coupling Factors** k p 0.58 0.57 0.57 0.65 0.56 0.62 0.59 0.64 0.55<br />

k 31 0.34 0.33 0.33 0.37 0.32 0.39 0.33 0.37 0.30<br />

k 33 0.70 0.68 0.68 0.72 0.65 0.72 0.70 0.75 0.68<br />

k t 0.50 0.50 0.47 0.51 0.47 0.50 0.47 0.52 0.48<br />

<strong>Piezo</strong>electric Charge Constants -d 31 [10 -12 C/N] 140 130 130 195 150 260 170 240 100<br />

d 33 [10 -12 C/N] 320 310 290 460 360 670 425 575 240<br />

<strong>Piezo</strong>electric Voltage Constants -g 31 [10 -3 Vm/N] 11 11 11 13 9 9 11 10 11<br />

g 33 [10 -3 Vm/N] 27 25 28 27 23 19 27 23 27<br />

Frequency Constants N E p [m/s] 2160 2280 2230 1940 2180 1970 2010 1970 2270<br />

N D t [m/s] 1980 2000 2040 2010 2040 1990 1950 1960 2050<br />

N E 1 [m/s] 1470 1600 1500 1400 1400 1410 1610<br />

N D 3 [m/s] 1340 1500 1800 1390 1500 1500 1500<br />

PHYSICAL PROPERTIES (tolerances +/- 5%)<br />

Mechanical Quality Factor Q m 700 1400 >1000 80 80 70 80 90 1000<br />

Density ρ [10 3 kg/m 3 ] 7.75 7.90 7.70 7.80 7.60 8.00 7.70 7.45 7.80<br />

Elastic Compliances s E 11 [10 -12 m 2 /N] 13 13 13 16 16 17 17 17 11<br />

s E 33 [10 -12 m 2 /N] 17 16 20 19 18 21 23 23 14<br />

Curie Temperature T c [°C] 325 290 330 340 340 170 350 235 305<br />

*) For multilayer components only.<br />

**) Measured in accordance with standard EN 50324.<br />

The values listed above are for reference purposes only and cannot be applied unconditionally to other shapes and<br />

dimensions. Values vary depending on the components' actual shape, surface finish, shaping process and post-processing.<br />

www.noliac.com <strong>Piezo</strong> <strong>ceramics</strong> Ver0901 2

<strong>Piezo</strong> <strong>ceramics</strong><br />

<strong>Piezo</strong> <strong>ceramics</strong> characteristics<br />

<strong>Piezo</strong>electric <strong>ceramics</strong> have the property of developing an electric charge when mechanical stress is exerted on them.<br />

In these materials, an applied electric field produces a proportional strain. The electrical response to mechanical<br />

stimulation is called the direct piezoelectric effect, and the mechanical response to electrical stimulation is called the<br />

converse piezoelectric effect.<br />

<strong>Piezo</strong>electric <strong>ceramics</strong> are usually divided into two groups. The antonyms “hard” and “soft” doped piezoelectric <strong>ceramics</strong><br />

refer to the ferroelectric properties, i.e. the mobility of the dipoles or domains and hence also to the polarization/<br />

depolarization behaviour.<br />

Hard doped piezoceramic materials<br />

Hard doped PZT materials can be exposed to high electrical and mechanical stresses. The stability of their properties<br />

makes them ideal for high-power applications.<br />

<strong>Piezo</strong>ceramic materials NCE41 and NCE40 are low loss materials for high power applications. The low dielectric and<br />

mechanical losses (tan(δ), Qm) combined with high piezoelectric charge constant (d 33 ) make them suitable for highperformance<br />

ultrasonic applications.<br />

Furthermore NCE41 and NCE40 can be exposed to high repetitive quasi-static and dynamic loads for ignition applications.<br />

NCE41 and NCE40 differ from each other in permittivity and mechanical quality factor values. This variability enables to<br />

fulfil all specific requirements.<br />

<strong>Piezo</strong>ceramic material NCE80 is intended for power transducers with highest electric drive. Its low dielectric and mechanical<br />

losses at extremely high electric drive and high coupling factors make it suitable for high-power applications.<br />

Soft doped piezoceramic materials<br />

Soft doped piezoelectric <strong>ceramics</strong> are distinguished by a comparatively high domain mobility and thus “ferro electrically<br />

soft” behaviour, i.e. relatively easy polarization.<br />

These materials are characterized by high relative permittivity, large electromechanical coupling factors, large piezoelectric<br />

constants and low mechanical quality factors. They are particularly suitable for sensing applications, receivers,<br />

actuators and low power transducers.<br />

<strong>Piezo</strong>ceramic materials NCE51 and NCE57 are standard soft materials, particularly suitable for actuators and low power<br />

non- resonant applications in which high coupling factor and /or high charge sensitivity are requested.<br />

<strong>Piezo</strong>ceramic material NCE53 has slightly lower electro-mechanical coupling factor, but has the advantage of higher temperature<br />

stability, and it is suitable especially for shear mode vibration sensors.<br />

<strong>Piezo</strong>ceramic materials NCE55 and NCE59 are very high sensitivity materials featuring extremely high permittivity, large<br />

coupling factor and piezoelectric constant. They have a relatively low Curie temperature. These materials are suitable<br />

for a wide range of high sensitivity applications with limited temperature range of operation.<br />

www.noliac.com <strong>Piezo</strong> <strong>ceramics</strong> Ver0901 3

<strong>Piezo</strong> <strong>ceramics</strong><br />

Navy types - equivalences<br />

Hard materials<br />

Soft materials<br />

Material NCE40 NCE41 NCE46 NCE80 NCE51 NCE53 NCE55 NCE57 NCE59<br />

Navy Type I I I III II II VI II V<br />

European<br />

standard<br />

EN 50324-1<br />

100 100 100 100 200 200 600 200 600<br />

Technical piezo <strong>ceramics</strong> description<br />

<strong>Piezo</strong>electricity is the property of nearly all materials that have a non-centrosymmetric crystal structure.<br />

Some naturally occurring crystalline materials that possess these properties are quartz and tourmaline. Some artificially<br />

produced piezoelectric crystals are Rochelle salt, ammonium dihydrogen phosphate and lithium sulphate. Another class<br />

of materials possessing these properties is polarized piezoelectric ceramic. In contrast to the naturally occurring piezoelectric<br />

crystals, piezoelectric <strong>ceramics</strong> have a polycrystalline structure.<br />

The most commonly produced piezoelectric <strong>ceramics</strong> are lead zirconate titanate (PZT), barium titanate and lead titanate.<br />

Ceramic materials have several advantages over single crystals, especially the ease of fabrication into a variety of<br />

shapes and sizes. In contrast, single crystals must be cut along certain crystallographic directions, limiting the possible<br />

geometric shapes.<br />

PZT (and many other piezoelectric materials) have crystal structures belonging to the perovskite family with the general<br />

formula AB0 3 . In the following figure the ideal, cubic perovskite structure (centrosymme tric) and tetragonal (ferroelectric)<br />

structure are shown.<br />

A piezoelectric ceramic material consists of<br />

small grains (crystallites), each containing<br />

domains in which the polar direction of the unit<br />

cells are aligned. Before poling, these grains<br />

and domains are randomly oriented; hence the<br />

net polari zation of the material is zero, i.e. the<br />

ceramic does not exhibit piezoelectric properties.<br />

The application of a sufficiently high DC<br />

field (called poling process) will orient the<br />

domains in the field direction and lead to<br />

a remanent polarization of the material.<br />

Pb<br />

0<br />

Ti, Zr<br />

Fig.1 The Perovskite crystal structure.<br />

+<br />

The perovskite structure is very tolerant to element<br />

substitution (doping) by formation of solid<br />

solutions. The possibilities of doping in these materials lead to an unlimited number of possible perovskite-type oxides.<br />

Even small amounts of a dopant may cause huge changes in the properties of a material.<br />

The coupling of electrical and mechanical energy makes piezoelectric materials useful in a wide range of applications.<br />

www.noliac.com <strong>Piezo</strong> <strong>ceramics</strong> Ver0901 4

<strong>Piezo</strong> <strong>ceramics</strong><br />

Constitutive equations<br />

The piezoelectric effect depends on directions.<br />

The reference axis, called axis 3, is taken<br />

parallel to the direction of poling. Axes 1 and 2<br />

are defined arbitrarily in order to form a direct<br />

coordinate system with axis 3. 4, 5 and 6 represent<br />

shear movements around axes 1, 2 and 3<br />

respectively.<br />

<strong>Piezo</strong>electric coefficients<br />

Based on this coordinate system, the piezoelectric<br />

effect can be described in a simplified<br />

way by matrix coefficients. The coefficients “d”<br />

(piezoelectric change constant 3×6 matrix) and<br />

“s E ” (elastic compliance 6×6 matrix) are commonly<br />

used.<br />

Fig.2 Electric dipoles in piezoelectric materials before, during and<br />

after poling.<br />

+<br />

—<br />

Basic piezoelectric equations<br />

These coefficients are used to relate the strain<br />

“S” (6-components tensor) to the stress “T”<br />

(6-components tensor) and electrical field “E”<br />

(3-components vector).<br />

3<br />

6<br />

S = s E .T + d.E<br />

Polarization<br />

In this equation, the “s E .T” term describes the<br />

mechanical compliance of the component, similarly<br />

to any mechanical component. The “d.E”<br />

term describes the piezoelectric effect, i.e.<br />

strain generated by electrical field.<br />

5<br />

2<br />

The above equations are useful for designing a<br />

piezoelectric application. However, it must be<br />

kept in mind that they represent an approximation.<br />

1<br />

4<br />

Fig.3 Designation of axes in piezoelectric materials.<br />

www.noliac.com <strong>Piezo</strong> <strong>ceramics</strong> Ver0901 5

<strong>Piezo</strong> <strong>ceramics</strong><br />

Definition of piezoelectric properties<br />

Properties Symbol / Definition Dimension<br />

ELECTRICAL PROPERTIES<br />

Relative Dielectric Constant<br />

(at 1V/1kHz)<br />

Dielectric Loss Factor<br />

K T = εT<br />

ε 0<br />

with<br />

ε T =permittivity (F/m)<br />

ε 0 =permittivity of free space (8.854 × 10 -12 F/m)<br />

K 3<br />

T<br />

tan(δ) =<br />

All stresses on material are constant or no external forces<br />

Electrodes are perpendicular to 3 axis<br />

Effective series resistance<br />

Effective series reactance<br />

1<br />

ELECTROMECHANICAL PROPERTIES<br />

Electromechanical<br />

Coupling Factors<br />

k =<br />

Mechanical energy stored<br />

Electrical energy applied<br />

=<br />

Electrical energy stored<br />

Mechanical energy applied<br />

k 31<br />

k 33<br />

Applied stress, or the piezoelectrically induced strain, is in 1 direction<br />

Electrodes are perpendicular to 3 axis<br />

Applied stress, or piezoelectrically induced strain, is in 3 direction<br />

Electrodes are perpendicular to 3 axis<br />

1<br />

1<br />

<strong>Piezo</strong>electric Charge<br />

Constants<br />

d =<br />

Strain developed<br />

Applied field<br />

=<br />

Charge density<br />

Applied stress<br />

d 31<br />

d 33<br />

Applied stress, or the piezoelectrically induced strain, is in 1 direction<br />

Electrodes are perpendicular to 3 axis<br />

Applied stress, or piezoelectrically induced strain, is in 3 direction<br />

Electrodes are perpendicular to 3 axis<br />

C/N<br />

C/N<br />

<strong>Piezo</strong>electric Voltage<br />

Constants<br />

g =<br />

Strain developed<br />

Applied charge density<br />

=<br />

Field developed<br />

Applied mechanical stress<br />

g 31<br />

g 33<br />

Applied stress, or the piezoelectrically induced strain, is in 1 direction<br />

Electrodes are perpendicular to 3 axis<br />

Applied stress, or piezoelectrically induced strain, is in 3 direction<br />

Electrodes are perpendicular to 3 axis<br />

Vm/N<br />

Vm/N<br />

www.noliac.com <strong>Piezo</strong> <strong>ceramics</strong> Ver0901 6

<strong>Piezo</strong> <strong>ceramics</strong><br />

Properties Symbol / Definition Dimension<br />

Frequency Constants<br />

N = F.X<br />

With F = resonance frequency (Hz)<br />

X = dimension governing the resonance (m)<br />

m/s<br />

N E p<br />

Planar mode, disc<br />

Measured with closed circuit<br />

m/s<br />

N E l<br />

Transverse mode, thin bar<br />

Measured with closed circuit<br />

m/s<br />

N D 3<br />

Longitudinal mode, cylindar<br />

Measured with closed circuit<br />

m/s<br />

Elastic Compliances<br />

s = 1 Y<br />

=<br />

Strain<br />

Stress<br />

with Y = Young modulus<br />

s E<br />

10 -12 m 2 /N<br />

11<br />

Compliance is measured with closed circuit<br />

Stress or strain is in 1 direction<br />

Strain or stress is in 1 direction<br />

s E<br />

10 -12 m 2 /N<br />

33<br />

Compliance is measured with closed circuit<br />

Strain or stress is in 3 direction<br />

Stress or strain is in 3 direction<br />

Curie Temperature T c<br />

°C<br />

www.noliac.com <strong>Piezo</strong> <strong>ceramics</strong> Ver0901 7